- Nano Express
- Open Access
Bi5FeTi3O15 nanofibers/graphene nanocomposites as an effective counter electrode for dye-sensitized solar cells
Nanoscale Research Letters volume 12, Article number: 18 (2017)
The present study reports Bi5FeTi3O15 (BFTO) nanofibers/graphene (Gr) nanocomposites (BGr) as counter electrodes (CEs) in dye-sensitized solar cells (DSSCs). BFTO nanofibers with diameters of 40–100 nm were fabricated by sol-gel based electrospinning technique. The microstructure and surface morphology of the BFTO nanofibers and the BGr nanocomposites were characterized by X-ray diffraction, scanning electron microscopy and transmission electron microscopy. The electrochemical performances of BGr CEs were comprehensively characterized and investigated. Compared to pristine BFTO, the nanocomposites have a marked improvement in electrocatalytic performance for the reduction of triiodide because of larger surface area and lower transfer resistance on the electrolyte-electrode interface. The maximum power conversion efficiency has reached 9.56%, which is much larger than that of pure BFTO CEs (0.22%).
In recent years, dye-sensitized solar cells (DSSCs) have attracted extensive attention as a potential alternative to silicon solar cells due to its high efficiency and low cost . As a rule, the DSSC consists of three parts: a dye-sensitized TiO2 photoanode, an electrolyte including iodide/triiodide (I3 ─/I─) redox couples, and a counter electrode (CE) with excellent catalytic ability . In general, the CE plays an important role in collecting the electron from an external circuit to catalyze the reduction of triiodide (I3 ─) to iodide (I─) in a DSSC [3, 4]. Consequently, the ideal CE material needs to have a high reduction catalytic activity, good chemical stability, low sheet resistance, and low production cost [5, 6]. Platinum (Pt) has been widely used as an ideal material for CE, however, the expensive price and limited reserves in nature have been the major concern for the energy community. Therefore, exploring replace Pt-based CE material in DSSC has attracted the attention of research institutions [7, 8].
Graphene (Gr) and its hybrids, which rely on their high thermal conductivity, excellent mobility of charge carriers, and extremely high theoretical specific surface area, have been widely used as CEs in DSSCs [9–11]. Recently, some materials including carbon nanotubes, poly(3,4-ethylenedioxythiophene), ZnO, TiO2, and NiCo2O4 composited with graphene have shown improved electrochemical behavior and power conversion efficiency compared to those without graphene [12–16]. But quaternary metal oxide Bi5FeTi3O15/grapheme composites have been rarely mentioned in previous literatures for DSSCs.
Bi5FeTi3O15 (BFTO) is a member of perovskite family, which exhibits a variety of interesting physical properties containing magnetic, ferroelectric, and dielectric properties [17–19]. BFTO is a kind of material with a direct bandgap (2.13 eV), high chemical stability and non-toxicity [20–22]. BFTO can be gained by inserting BiFeO3 into three-layered Bi4Ti3O12, forming a four-layered perovskite structure . Bi4Ti3O12 and BiFeO3 have been found to be good candidates for DSSC [24, 25]. As a result, BFTO could also be utilized to build DSSCs. However, these ferroelectric oxides as CE in DSSC have scarcely been reported. In this work, we demonstrated BFTO/Gr nanocomposites as CE in DSSCs due to the low charge mobility and inferior catalytic activity of BFTO CE, expecting that Gr could promote the catalytic activity of the nanocomposites CE and thus enhance the photovoltaic property of the DSSCs based on the BFTO. This work could widen the potential applications of multibasic oxides in the photophysics and photochemistry field.
All chemicals except graphene are of analytical grade. High purity (99.5%) graphene was purchased from Aladdin Industrial Corporation. Firstly, ethanol, bismuth nitrate, and iron acetylacetonate were dissolved in N, N-dimethylformamide. Then, tetrabutyl titanate and polyvinylpyrrolidone were slowly added in the solution stirring for 12 h to form the yellow precursor solution for electrospinning. The electrospinning parameters were setted as accelerating voltage of 10 kV and collecting distance of 20 cm, and the as-collected nanofibers were calcined in muffle furnace at 650 °C.
The TiO2, used as photoanode, was soaking through N719 dye-sensitized solution and dried in air. BFTO or BFTO/graphene (BGr) powder (0.1 g) was mixed in appropriate amount of PEG 2000 and ground constantly. Then, absolute ethanol (1 ml) was added and stirred to form a colloid. The CEs were gained by coating on FTO glass with the colloid followed by heating at 400 °C for 30 min under the protection of argon. BGr CEs were prepared with Gr of 0, 0.5, 1, 1.5 and 2 wt%, (labeled as BGr0, BGr0.5, BGr1, BGr1.5, BGr2), respectively. The effective areas of all cells were 0.25 cm2. Finally, the DSSC was assembled with prepared TiO2 photoanode like sandwich structure and was injected the electrolyte into the internal space between CE and photoanode.
A diffractometer with a Cu-Kα (with λ = 0.1542 nm) radiation source was used as the record of X-ray diffraction (XRD DX-2700) pattern for structures characterizing. The surface morphologies and microstructures were observed by using a scanning electron microscope (SEM, JSM-7001 F) and transmission electron microscope (TEM, JEM-2100). The electronic absorption spectra were recorded by a UV-vis photospectrometer (Varian Cary 5000). The photocurrent-voltage (J-V) curves of the DSSCs were recorded by a solar simulator under AM 1.5 illumination. The J-V curves, electrochemical impendence spectroscopy (EIS) and Tafel polarization curves were characterized by the electrochemical workstation (Wuhan CorrTest Instrument Co., Ltd.). Monochromatic incident photo-to-current conversion efficiency (IPCE) curves of devices were measured on an IPCE measurement system (Qtest Station 500ADX). The fill factor (FF) and the photoelectric conversion efficiency (η) of DSSC are calculated according to the following equations:
Where J sc is the short-circuit current density (mA cm−2), V oc is the open-circuit voltage (V), P in is the incident light power (mW cm−2), and J max (mA cm−2), and V max (V) is the current density and voltage at the point of the maximum power output in the J-V curves, respectively.
Results and discussion
Figure 1a presents the XRD patterns of pure BFTO nanofibers, Gr powders, and BGr nanocomposites, respectively. The positions and relative intensities of diffraction peaks are corresponding to JCPDS card NO.38-1257 and 65-6212, which indicate that the BFTO and Gr are pure phase within the limitation of XRD diffractometer, respectively. It is noted that the XRD patterns of BGr0.5, BGr1, BGr1.5, and BGr2 are almost the same and the peaks of Gr are not observed due to its less content. Raman spectra are shown in Fig. 1b and c to further verify the phase composition of the samples. For BFTO, the 260, 321, 534, and 857 cm−1 modes are resulted from the torsional bending and the stretching vibration modes of TiO6 octahedral. The origin of 715 cm−1 mode should be correlated to the Bi-Fe-O perovskite block because this mode has not been found in some Bi-layered oxides without Fe element such as Bi4Ti3O12 and CaBi4Ti4O15 [26, 27]. Moreover, the mode at 321 cm−1 could correspond to ferroelectric phase transition as reported previously . From the Raman measurement result, it is reasonable to conclude that BFTO single phase with four-layered perovskite structure has been successfully prepared. As seen from Fig. 1c, there are two prominent peaks of Gr at 1339 and 1583 cm−1, which are assigned to the disordered (D) and graphitic (G) bands, respectively. The D peak is due to edge planes and disordered structure defect of lattice, while G peak belongs to the E 2g phonon of sp2 bonded carbon atoms [29, 30]. Consequently, the BFTO and Gr are successfully composited from the above Raman spectrum. Although 2D band is characteristic peak for graphene in Raman spectrum, in some literatures for graphene composited with inorganics, no 2D band was observed [31–33]. Moreover, in the references 15 and 31, the Raman measurement of graphene shows that the intensity of D-band (I D) is relatively higher than that of G-band (I G), while I G is larger than that of I D for the graphene oxide .
Figure 1d shows the UV-vis spectra of the BFTO, BGr, and Gr. According to the spectrum of BFTO, it could find that BFTO absorbs light from UV light to visible light shorter than 600 nm, which is consistent with its yellow appearance. According to the UV-vis spectra, the Gr has a perfect photoabsorption property in the whole visible light region. Therefore, BFTO compounded with Gr could display a better light-harvesting capability over the visible to near-IR region, which is also ascertained by the UV-vis spectra of BGr nanocomposites. The (αhv)1/2 versus hv plots are shown in Fig. 1e. By means of linear extrapolation method, the optical bandgap of BFTO nanofibers can be approximately estimated as 2.13 eV, which is comparable with that published in the previous literature. Moreover, it can be seen that optical bandgap of BGr decreases with increasing Gr content, which indicates the photoabsorption ability and the numbers of photogenerated carriers can be increased through the combination of Gr.
The surface morphology and microstructure of BFTO nanofibers, BGr, and Gr are presented in Fig. 2. From Fig. 2a, the average diameter of the unsintered nanofibers is in the range of 100–300 nm, and their surface are smooth. After calcination, a continuous fine grained structure was observed and the average diameter of BFTO fibers is in the range of 40–100 nm. The SEM images of BFTO, Gr, and BGr films as CEs are displayed in Fig. 2c–e, respectively. It is obvious that the BFTO and Gr CEs are composed of nanoparticles and thin silk-like sheets. As shown in Fig. 2e, Gr sheets are commendably dispersed with the BFTO nanoparticles, which indicate the BGr nanocomposites have been successfully synthesized. The TEM image of typical BGr sample is exhibited in Fig. 2f, the black particles characterize the BFTO nanoparticles, and the reticulation denotes gray Gr. It can be inferred that BFTO and Gr are adequately mixed without change in crystalline structure. According to the high magnification TEM image in Fig. 2g, h, the lattice spacing is measured to be about 0.295 and 0.335 nm by the formula of Rd = L, matching with the (119) plane of orthorhombic BFTO and (002) reflection of Gr, respectively. This can be further confirmed by the selected area electron diffraction (SAED) image of typical BGr in Fig. 2i, which appears as the strong diffraction spots of BFTO and the diffraction rings of Gr.
EIS measurement is performed in symmetrical cells fabricated with two identical CEs (CE/electrolyte/CE) to analyze the correlation between the electrocatalytic activity of the CE and quality of devices. Nyquist plots in Fig. 3a–c, and d clarify impedance characteristics of the DSSCs based on BGr0, BGr0.5, BGr1, BGr1.5, BGr2, Gr, and Pt CEs; and the corresponding electrochemical parameters are summarized in Table 1. The intercept on the horizontal axis stands for the series resistance (R s), a reflection of conductive substrate resistance, and lead resistance. The charge transfer resistance (R ct) at the CE/electrolyte interface is the intercept of the first semicircle, which characterizes the electrocatalytic ability of CEs for the reduction of triiodide , while the Nernst diffusion impedance corresponding to the diffusion resistance of the redox couples in the electrolyte is referred by the second arc. It is worthwhile to note that R ct and R s are the important parameters for appraising the performance of CEs. It is well known that a smaller R s represents a higher conductivity and the smaller R ct, the lower ∆E p, bringing about a faster electron transfer from CE to electrolyte, thus the electrocatalytic activity can be enhanced. From Table 1, the R s of BGr2 and BGr0 is 7.81 and 8.77 Ω cm2, respectively. Meanwhile, it is also observed that BGr0 and BGr0.5 have much larger R ct, implying that BGr0 and BGr0.5 have poor electrocatalytic ability. The R ct of BGr2 is 0.82 Ω cm2, comparable with that of the reference Pt electrode (0.73 Ω cm2), indicating that BGr2 nanocomposite has an excellent electric conductivity and catalytic activity, which is an attribute to large specific surface area and high conductivity of BGr2 CE sample. Furthermore, the R ct value for the BGr2 CE is much smaller than that of BGr0 CE, indicating that the former CE possesses more excellent catalytic activity and superior conductivity for I 3 ─ reduction than pristine BFTO CE. In addition, it is clearly seen that the R ct and R s of the BTO/Gr CE are becoming smaller with increasing concentration of Gr, which presumably derives from the lamellar structure of graphene effectively promoting the electron transport and the diffusion of the redox electrolyte within the CEs, further resulting in better catalytic activity.
Tafel polarization curves are used to further investigate the catalytic activity of various CEs. As indicated in Fig. 4a, the exchange current density (J 0) is approximately calculated by Tafel linear extrapolation method, namely, the intersection of the cathodic branch and the equilibrium potential line. The limiting current density (J lim) depends on the intersection of the cathodic branch and the vertical axis. The J 0 and J lim are closely related to the catalytic activity of catalysts, which can severally assess the reduction capability and the diffusion capability of the iodide/triiodide redox couple on CE materials . Generally, a larger slope implies a higher J 0. Obviously, the catalytic ability of various CEs is in the order of Pt > Gr > BGr2 > BGr1.5 > BGr1 > BGr0.5 > BGr0, suggesting that Gr is favorable for increasing the interfacial contact and decreasing the charge recombination rate by providing fast electron transport at CEs/electrolytes interfaces, thus enhancing the catalytic capability of pure BFTO CE for the reduction of triiodide, which is in consistent with the previous EIS results. Tafel polarization measurements further ascertain that Gr indeed improves the conductive ability and directly influences electrocatalytic activity of BFTO.
Figure 4b presents the IPCE of the DSSCs assembled with the assorted CEs. It can be seen that the strong photoelectric responses of DSSC with various CEs are all located at about 510 nm, and the photoelectric response enhances with the increasing of Gr content, which may probably due to the increased photogenerated carrier numbers originated from the increasing light absorption. The maximum photoelectrical responses of IPCE for the devices based on the BGr0 and BGr2 CEs are 8.3 and 42.3%, respectively. Since the values of IPCE are chiefly responsible by dye loading capacity and electron collection efficiency, it can be apparently distinguished that after Gr incorporation, more active sites are produced for the absorption of dye molecules and the photocurrent in the external circuit is enhanced, which increases the charge collection efficiency. As a result, the BFTO/Gr CEs have a faster electron transmission and a higher dye absorption capacity. Furthermore, the variation trend of the IPCE measurement is in a good consistent with the prior EIS results [37–39].
The J-V curves for the DSSCs fabricated with various CEs are shown in Fig. 4c, and the detailed photovoltaic parameters estimated from the J-V curves, including open-circuit voltage (V oc), short-circuit current density (J sc), fill factor (FF), and power conversion efficiency (PCE) are also summarized in Table 1. The photovoltaic parameters of DSSCs are gradually eased with increasing Gr content. When the mass fraction of Gr exceeds 2%, the PCE of DSSC remains nearly constant based on numerous photoelectric performance measurements. It is found that the DSSC assembled by BGr2 gives a PCE of 9.56%, V oc of 740 mV, J sc of 21.56 mA/cm2, and FF of 0.599, which is forty times greater than that of the DSSC based on the pristine BFTO CE (PCE = 0.22%, V oc = 0.364 V, J sc = 3.8 mA/cm2, and FF = 0.159). Consequently, Gr can advance the electrocatalytic activity of the BFTO CE which is in line with the former tests (EIS and Tafel curves). The improved photovoltaic performance of the DSSCs after Gr incorporation mainly ascribes to the following aspects: The contact frequency between the redox couple in electrolyte and the electrode can be accelerated owning to the large specific surface area of Gr, thus improve the electrolyte absorption ability and reaction speed. Then, the BGr CEs exhibit an improved electrocatalytic activity and electrolyte/electrode contact area compared with that of pure BFTO CE, leading to fast reaction kinetics and offering more electrocatalytic sites for the reduction of I3 − at the CE/electrolyte and a low charge recombination. Our study clearly demonstrates that small amount of Gr can significantly improve the electrochemical and photovoltaic properties of BFTO. Although the PCE value of BGr2 CE (9.56%) is smaller than that of Pt CE (12.21%), our work suggest that the incorporation of BFTO with Gr could be a promising and effective alternative to the noble Pt metal as a CE in DSSCs. Most recently, Gr are widely used to improve the photoelectrochemical properties of some metal oxides such as La0.65Sr0.35MnO3 and ZnO [40, 41], to our knowledge, it is the first time to describe Gr enhancing electrocatalytic activity and photovoltaic performance for four-component ferroelectric oxides.
Figure 4d, e shows the cyclic voltammetry (CV) curves of various BFTO based CEs, which is measured by using a three-electrode system with the Pt sheet as CE, saturated sliver chloride electrode as reference electrode, and various CEs as working electrode. For comparison, the CV curves for Pt and Gr are also displayed in Fig. 4d. Generally, a smaller overpotential (E pp) represents a better catalytic activity . From Fig. 4d, e, the BGr2 CE has the lowest E pp value among all BFTO-based CEs, reflecting that BGr2 CE has a decent catalytic activity. This is mainly due to Gr possesses a larger specific surface area which can hugely enhance the assessibility of the electrolyte to the electrode, thus improving interfacial charge transfer and enhancing the number of active catalytic sites, which is also complied with by the foregoing EIS, IPCE, and J-V measurement results. Moreover, 20 cycles of CV curves in Fig. 4f are employed to illustrate the stability of BG2 CE. It makes clear that BGr2 CE is fairly stable for catalyzing triiodide. The above experimental results imply that the incorporation of Gr can indeed improve the catalytic activity of BTO.
In conclusion, Bi5FeTi3O15/graphene (BFTO/Gr) CEs have been successfully synthesized by a facile approach based on sol-gel and electrospinning techniques. The structure and morphology of the CEs were characterized by X-ray diffraction, scanning electron microscopy, and transmission electron microscopy. Extensive experiments indicate that BFTO/Gr CE has a vast enhancement of photovoltaic performance in comparison with pristine BFTO CE, which express as higher catalytic activity for the reduction of triiodide, larger specific surface area, and lower charge transfer resistance on the electrolyte-electrode interface, in which Gr plays a key role due to its inherent features. Under the optimum conditions, the largest PCE reaches 9.56% for the BGr2 CE in the DSSCs, which is 40 times larger than that of pure BFTO CE. This work provides a new, simple and effective means to improve the photoresponsivity of commonly four-component ferroelectric oxides, which may develop the application area of multifunctional metal oxides.
BFTO nanofibers/Gr nanocomposites
Dye-sensitized solar cells
Electrochemical impendence spectroscopy
- I D :
The intensity of D-band
- I G :
The intensity of G-band
Monochromatic incident photo-to-current conversion efficiency
- J-V :
Scanning electron microscope
Transmission electron microscope
- η :
Photo-electric conversion efficiency
Yue GT, Ma XP, Zhang WF, Li FM, Wu JH, Li GQ (2015) A highly efficient flexible dye-sensitized solar cell based on nickel sulfide/platinum/titanium counter electrode. Nanoscale Res Lett 10:1
Liu WQ, Kou DX, Cai ML, Hu LH, Sheng J, Tian HJ, Jiang NQ, Dai SY (2010) The intrinsic relation between the dynamic response and surface passivation in dye-sensitized solar cells based on different electrolytes. J Phys Chem C 114:9965–9969
Hauch A, Georg A (2001) Diffusion in the electrolyte and charge-transfer reaction at the platinum electrode in dye-sensitized solar cells. Electrochim Acta 46:3457–3466
Mohamed IMA, Motlak M, Akhtar MS, Yasin AS, EI-newehy MH, Al-Deyab SS, Barakat NAM (2016) Synthesis, characterization and performance as a Counter Electrode for dye-sensitized solar cells of CoCr-decorated carbon nanofibers. Ceram Int 42:146–153
Yeh MH, Chang SH, Lin LY, Chou HL, Vittal R, Hwang BJ, Ho KC (2015) Size effects of platinum nanoparticles on the electrocatalytic ability of the counter electrode in dye-sensitized solar cells. Nano Energy 17:241–253
Kaniyoor A, Ramaprabhu S (2012) Enhanced efficiency in dye sensitized solar cells with nanostructured Pt decorated multiwalled carbon nanotube based counter electrode. Electrochimi Acta 79:199–206
Yan Y, Wang JZ, Chang QH, Babikier M, Wang HX, Li HT, Yu QJ, Gao SY, Jiao SJ (2013) Fabrication of mesoporous TiO2 electrodes by chemical technique for dye-sensitized solar cells. Electrochim Acta 94:277–284
Yan Y, Wang JZ, Wang WQ, Sun JM, Wang DB, Li Q, Babikier M, Wang HX, Yu QJ, Jiao SJ, Gao SY, Li HT (2013) Separation of anatase phase from commercially available P25 powder for dye-sensitized solar cells. Electrochim Acta 114:681–687
Chen JK, Li KX, Luo YH, Guo XZ, Li DM, Deng MH, Huang SQ, Meng QB (2009) A flexible carbon counter electrode for dye-sensitized solar cells. Carbon 47:2704–2708
Allen MJ, Tung VC, Kaner RB (2010) Honeycomb carbon: a review of graphene. Chem Rev 110:132–145
Yue GT, Li FM, Yang G, Zhang WF (2016) Efficient nickel sulfide and graphene counter electrodes decorated with silver nanoparticles and application in dye-sensitized solar cells. Nanoscale Res Lett 11:239
Chen PY, Li CT, Lee CP, Vittal R, Ho KC (2015) PEDOT-decorated nitrogen-doped graphene as the transparent composite film for the counter electrode of a dye-sensitized solar cell. Nano Energy 12:374–385
Kim H, Choi H, Hwang S, Kim Y, Jeon M (2012) Fabrication and characterization of carbon-based counter electrodes prepared by electrophoretic deposition for dye-sensitized solar cells. Nanoscale Res Lett 7:53
Jang HD, Jo EH, Chang H, Kim J, Roh KM (2015) Incorporation of 3D crumpled graphene in nanostructured TiO2 films for dye-sensitized solar cells. Mater Lett 142:304–307
Chang QH, Ma ZJ, Wang JZ, Yan Y, Shi WZ, Chen Q, Huang YW, Yu QJ, Huang L (2015) Graphene nanosheets@ZnO nanorods as three-dimensional high efficient counter electrodes for dye sensitized solar cells. Electrochim Acta 151:459–466
Yue GT, Yang G, Li FM, Wu JH (2015) PEDOT: PSS assisted preparation of a graphene/nickel cobalt oxide hybrid counter electrode to serve in efficient dye-sensitized solar cells. RSC Adv 5:100159–100168
Li J, Huang Y, Rao G, Liu G, Luo J, Chen J, Liang J (2010) Ferroelectric transition of Aurivillius compounds Bi5Ti3FeO15 and Bi6Ti3Fe2O18. Appl Phys Lett 96:222903
Mao X, Wang W, Chen X, Lu Y (2009) Multiferroic properties of layer-structured Bi5Fe0.5Co0.5Ti3O15 ceramics. Appl Phys Lett 95:082901
Zhao YW, Fan HQ, Liu GC, Liu ZY, Ren XH (2016) Ferroelectric, piezoelectric properties and magnetoelectric coupling behavior in aurivillius Bi5Ti3FeO15 multiferroic nanofibers by electrospinning. J Alloy Compd 675:441–447
Elzbieta J, Tomasz P, Karol K, Jolanta D, Piotr G, Dionizy C (2016) Magnetoelectric effect in ceramics based on bismuth ferrite. Nanoscale Res Lett 11:234
Qiu YD, Zhao SF, Wang ZP (2016) Magnetoelectric effect of Dy doped Bi5Ti3FeO15 films prepared by sol-gel method. Mater Lett 170:89–92
Yin WH, Chen C, Bai W, Yang J, Zhang YY, Tang XD, Duan CG, Chu JH (2016) Dielectric behavior dependence on temperature and Cr-doping contents of Aurivillius Bi5Ti3FeO15 ceramics. Cearm Int 42:4298–4305
Kubel F, Schmid H (1992) X-ray room temperature structure from single crystal data, powder diffraction measurements and optical studies of the Aurivillius phase Bi5(Ti3Fe)O15. Ferroelectrics 129:101–112
Chen Z, Li S, Zhang W (2011) Dye-sensitized solar cells based on Bi4Ti3O12. Int J Photoenergy 2011:821045
Lotey GS, Verma N (2014) Synthesis and characterization of BiFeO3 nanowires and their applications in dye-sensitized solar cells. Mat Sci Semicon Proc 21:206–211
Zhong XL, Wang JB, Liao M, Huang GJ, Xie SH, Zhou YC, Qiao Y, He JP (2007) Multiferroic nanoparticulate Bi3.15Nd0.85Ti3O12–CoFe2O4 composite thin films prepared by a chemical solution deposition technique. Appl Phys Lett 90:152903
Zhang ST, Chen YF, Liu ZG, Ming NB, Wang J, Cheng GX (2005) Structures and electrical properties of Bi5FeTi3O15 thin films. J Appl Phys 97:104106
Mao XY, Sun H, Wang W, Lu YL, Chen XB (2012) Effects of Co-substitutes on multiferroic properties of Bi5FeTi3O15 ceramics. Solid State Commun 152:483–487
Huang L, Chang QH, Guo GL, Liu Y, Xie YQ, Wang T, Ling B, Yang HF (2012) Synthesis of high quality graphene films on nickel foils by rapid thermal chemical vapor deposition. Carbon 50:551–556
Wu C, Huang XY, Wang GL, Lv LB, Chen G, Li GY, Jiang PK (2013) Highly conductive nanocomposites with three-dimensional, compactly interconnected graphene networks via a self-assembly process. Adv Funct Mater 23:506–513
Gong F, Li ZQ, Wang H, Wang ZS (2012) Enhanced electrocatalytic performance of graphene via incorporation of SiO2 nanoparticles for dye-sensitized solar cells. J Mater Chem 22:17321–17327
Bai S, Shen XP (2012) Graphene-inorganic nanocomposites. RSC Adv 2:64–98
Madhavan AA, Kalluri S, Chacko DK, Arun TA, Nagarajan S, Subramanian KRV, Nair AS, Nair SV, Balakrishnan A (2012) Electrical and optical properties of electrospun TiO2-graphene composite nanofibers and its application as DSSC photo-anodes. RSC Adv 2:13032–13037
Zheng HJ, Ni DJ, Yu Z, Liang P (2017) Preparation of SERS-active substrates based on graphene oxide/silver nanocomposities for rapid zdetection of L-Theanine. Food Chem 217:511–516
Fabregat-Santiago F, Bisquert J, Palomares E, Otero L, Kuang D, Zakeeruddin SM, Grätzel M (2007) Correlation between photovoltaic performance and impedance spectroscopy of dye-sensitized solar cells based on ionic liquids. J Phys Chem C 111:6550–6560
Ma DY, Guo HF, Qin L, Yue L, Ruan QT, Huang YW, Xu J (2014) Construction of a new 2D cadmium(II) coordination polymer based on N- and O-donor ligands: synthesis, luminescence and biological activities. J Chem Crystallogr 44:63–69
Cho S, Hwang SH, Kim C, Jang J (2012) Polyaniline porous counter-electrodes for high performance dye-sensitized solar cells. J Mater Chem 22:12164–12171
Yella A, Lee H-W, Tsao HN, Yi C, Chandiran AK, Nazeeruddin MK, Diau E-W-G, Yeh C-Y, Zakeeruddin SM, Grätzel M (2011) Porphyrin-sensitized solar cells with cobalt (II/III)-based redox electrolyte exceed 12 percent efficiency. Science 334:629–634
Chen C, Xie Y, Ghafar A, Yoo SH, Cho SO (2011) Improved conversion efficiency of Ag2S quantum dot-sensitized solar cells based on TiO2 nanotubes with a ZnO recombination barrier layer. Nanoscale Res Lett 6:462
Jayabal P, Gayathri S, Sasirekha V, Mayandi J, Ramakrishnan V (2014) Preparation and characterization of ZnO/graphene nanocomposite for improved photovoltaic performance. J Nanopart Res 16:2640
Xiong KW, Li G, Jin C, Jin SW (2016) La0.65Sr0.35MnO3@RGO nanocomposites as an effective counter electrode for dye-sensitized solar cells. Mater Lett 164:609–612
Yao RY, Zhou ZJ, Hou ZL, Wang X, Zhou WH, Wu SX (2013) Surfactant-free CuInS2 nanocrystals: an alternative counter-electrode material for dye-sensitized solar cells. ACS Appl Mater Inter 5:3143–3148
This work was financially supported by NSFC (51372069, U1504625, U1504624, 11305046) and Program for Science and Technology Innovation Talents in Universities of Henan Province (14HASTIT038).
HZ wrote the manuscript. HZ, BM, and GY conceived and designed the study. XL, HZ, and YY participated in the device preparation. YY, XL, KW, BM, and GY were involved in the SEM, XRD, EIS, IPCE, JV, and CV analysis of the devices. CD, CP, and XZ helped to draft the manuscript. All authors read and approved the final manuscript.
The authors declare that they have no competing interests.
About this article
Cite this article
Zheng, H.W., Liang, X., Yu, Y.H. et al. Bi5FeTi3O15 nanofibers/graphene nanocomposites as an effective counter electrode for dye-sensitized solar cells. Nanoscale Res Lett 12, 18 (2017). https://doi.org/10.1186/s11671-016-1799-5
- Counter electrode
- Dye-sensitized solar cell